# Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains

Save this PDF as:

Size: px
Start display at page:

Download "Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains"

## Transcription

1 Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model a composite is represented as an assemblage of concentric cylinders. The core of this cylinder is a fibre and surrounding annulus is a matrix material. This model is called concentric cylinder assemblage (CCA) model. In this lecture we give the introduction and back ground of this model. The Lecture Contains Concentric Cylinder Assemblage (CCA) Model Background of CCA Model Analysis of Concentric Cylinders Home Work References file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_1.htm[8/18/2014 3:57:06 PM]

2 Concentric Cylinder Assemblage (CCA) Model As we know, the unidirectional fibrous composite has fibres embedded in matrix material. The fibres are, in general, cylindrical in nature. Thus, Hashin and Rosen [1] introduced a micromechanical model in which the composite is represented as an assemblage of concentric cylinders. The inner cylinder represents the fiber and outer annulus is matrix. The fibres are considered to be infinitely long cylinders and matrix is considered to be continuous. The model is shown in Figure 7.10(a). For each individual fibre of radius, there is associated an annulus of matrix material of inner radius and outer radius. The individual cylinder, thus formed, is called as a composite cylinder. This is shown in Figure 7.10 (b). It should be noted that the all cylinders do not have the same radii. The radii of each cylinder vary in a way such that they completely fill the composite volume. However, the ratio of the fiber cylinder to the outer radius of matrix cylinder is same for all cylinders. This leads to the fact that all composite cylinders have the same volume fractions. Further, the resulting material is transversely isotropic in nature. The advantage of this model is that analysis of one composite cylinder is sufficient to determine the four out of five effective elastic moduli of a transversely isotropic material. Figure 7.10: (a) Concentric cylinder assemblage model (b) composite cylinder and (c) homogeneous single cylinder file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_2.htm[8/18/2014 3:57:06 PM]

3 Background of CCA Model Here, we will relate five effective independent stiffness coefficients with the measurable effective engineering constants. In the following, for a transversely isotropic material we derive relations between the stiffness coefficients and engineering constants. The unidirectional fibrous composite is transversely isotropic in nature in plane perpendicular to fibre direction (or in plane perpendicular to the plane in which fibres are placed together). The stress strain relations for the transversely isotropic material in 23 plane is written as (7.148) Thus, there are five constants, and are independent constants. These constants define the effective properties of the composite. Note that in above relations tensorial shear strains are used. The relation between these independent constants and effective engineering constants can be given as follows: Consider an uniaxial stress state such that and.. Putting this in Equation (7.148) we can solve for the normal strains. The normal strains in terms of and are given as (7.149) From the first of the above equation, we can write (7.150) We define the effective axial modulus through following equation as (7.151) Comparing this equation with Equation (7.150) we can write for as file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_3.htm[8/18/2014 3:57:06 PM]

4 (7.152) file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_3.htm[8/18/2014 3:57:06 PM]

5 Similarly, we define the following the Poisson s ratios and as (7.153) Thus, using Equation (7.149), we get (7.154) The other engineering constants that can be directly related to the effective stiffness coefficients are (7.155) Equations (7.152), (7.154) and (7.155) are four equations with five effective stiffness constants. We need one more equation in effective stiffness constants that relates an effective engineering constant. Then we can solve for and in terms of effective engineering constants. We develop this equation as follows. Let us define the plane strain bulk modulus, to the state of strain corresponding (7.156) For this state of strain, from the constitutive equation in Equation (7.148) the normal stresses are given as (7.157) Let us define where (7.158) is defined as effective plane strain bulk modulus. Now, Equations (7.152), (7.154), (7.155) and (7.158) can be inverted to give (7.159) In the above exercise, the measurable properties are and. However, one can file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_4.htm[8/18/2014 3:57:06 PM]

6 measure the other engineering properties and express the effective stiffness coefficients. Let us consider that a uniaxial tension normal to the fibre direction is applied such that and. Putting this in Equation (7.148) we can solve for the normal strains. The normal strains in terms of and are given as (7.160) From the second of the above equation, we can write (7.161) file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_4.htm[8/18/2014 3:57:06 PM]

7 Now we define the effective Poisson s ratios and as (7.162) Thus, using Equation (7.149), we get (7.163) and (7.164) Further, from the symmetry consideration we have the following relations (7.165) and from the reciprocal relations (7.166) Thus, we can write the following useful relations as (7.167) Thus, if we know the effective engineering constants and, then we can find the effective stiffness coefficients for transversely isotropic material. Further, the remaining engineering constants can also be determined. The effective stiffness can be determined from the composite cylinder either using the concept of equivalence of strain energy or the basic definitions for each of the engineering property. For the equivalence of strain energy approach the strain energy of the composite cylinder must be equal to the strain energy of the single homogeneous cylinder. The strain energy in a given volume of the cylinder is given as (7.168) file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_5.htm[8/18/2014 3:57:07 PM]

8 In the case of a composite cylinder, the integral over volume extends over the volume of the core cylinder plus the volume of the annulus and in case of homogeneous cylinder it is over the one cylinder. It should be noted that both cylinder systems are subjected to same deformations. This approach can be complicated in the case of concentric cylinders as it involves both the geometry and elastic properties of two cylinders. In the following sections we derive the effective engineering constants using the CCA model and basic definitions of engineering properties as follows. In this, the concentric cylinders are axially loaded. The composite axial modulus can be defined as axial force divided by axial strain produced by this axial force. Further, in this loading the assumption is that no other stresses are applied and the cylinders are free to deform. file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_5.htm[8/18/2014 3:57:07 PM]

9 Analysis of Concentric Cylinders When the concentric cylinders are subjected to either an axial load or a uniform radial stress then there are no shear stresses produced. Further, in an infinite cylinder away from the ends, the stresses are independent of. For this state of stress, there will be one equilibrium equation given as (7.169) where, and are radial and circumferential stresses, respectively. For a cylindrical coordinate system with no shear stresses, we can write normal stresses for transversely isotropic material as (7.170) Similarly, for transversely isotropic fibre and isotropic matrix the normal stresses are given as (7.171) Now, we write the strain displacement relations in cylindrical coordinates as (7.172) where, and are axial, circumferential or tangential and radial displacements, respectively. Further, with no shear effects and axisymmetry the tangential displacement is zero. It should be noted that the stresses are not function of. Hence, the strains are independent of. Hence, the displacement can be a function of. However, can be function of and, at most, a linear function of. Hence, in the expression for strain there is partial derivative and not in the expression for. For the expression of we have the full derivative with respect to. Thus, the normal strains for the displacements in this case simplify to When these strain-displacement relations are used in stress-strain relations then the equilibrium equation in Equation (7.169) gives an ordinary differential equation in as file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_6.htm[8/18/2014 3:57:07 PM]

10 (7.173) file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_6.htm[8/18/2014 3:57:07 PM]

11 The solution to this equation is (7.174) Thus, the solution for fibre is (7.175) and the solution for the matrix is (7.176) The axial displacement in fibre and matrix can be determined by integrating the first of Equation (7.172) with respect to. In this equation the left hand side is independent of. Thus, (7.177) It should be noted that and are constants and and are the arbitrary constants of integration. The constants and and functions and are unknown. These can be determined from specific boundary conditions. The displacement in fibre as given in Equation (7.175) should be bounded when. This requires the condition that (7.178) Further, the displacements are continuous at the interface of fibre and matrix. This results in (7.179) Using Equation (7.178) and Equation (7.179), the continuity conditions become file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_7.htm[8/18/2014 3:57:07 PM]

12 (7.180) On equating the terms in and in the second of Equation (7.180), we get (7.181) This means that the strains in -direction in fibre and matrix are given by same function of. Further, the unknown constant in fibre and matrix is same. This constant, in fact, is the axial strain. Therefore, it is denoted as. file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_7.htm[8/18/2014 3:57:07 PM]

13 The third continuity condition required is the continuity of the stress component normal to the interface between the fibre and matrix, that is, (7.182) Using, Equation (7.171) and the unknown constants in above condition, we get (7.183) The unknown constants and (7.183) can be determined from the first of Equation (7.180) and Equation (7.183) along with additional equations that will result due to the application of specific load or deformation, which in turn will depend upon which of the engineering property is to be determined. Let us write the strain displacement relations for fibre and matrix using Equation (7.172) and Equation (7.175) through Equation (7.177). (7.184) Note that the strains in the fibre are spatially uniform. Using above relation in Equation (7.171) we get the stresses in fibre and matrix as (7.185) From the above equation, it is easy to see that like strains, the stresses are also spatially uniform in the fibre. Further, the radial and hoop/transverse stresses are identical for this case. file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_8.htm[8/18/2014 3:57:07 PM]

14 Home Work: 1. What is a CCA model? 2. Give a brief description of the background for CCA model. file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_9.html[8/18/2014 3:57:07 PM]

15 References: Z Hashin, BW Rosen. The elastic moduli of fibre-reinforced materials. J. Appl. Mech. 1964, Vol. 31, pp Z Hashin. Analysis of properties of fiber composites with anisotropic constituents. J. Appl. Mech. 1979, Vol. 46, pp RM Christensen. Mechanics of Composite Materials. Krieger Publishing Company, Florida, Z. Hashin: On elastic behaviour of fibre reinforced materials of arbitrary transverse phase geometry. J. Mech. Phys. Solids, 1965, Vol. 13, pp Z. Hashin: Analysis of composite materials-a survey. J. Mech. Phys. Solids, 1983, Vol. 50, pp YC Fung. Foundations of Solid Mechanics. Prentice Hall International, Inc., CT Herakovich. Mechanics of Fibrous Composites, John Wiley & Sons, Inc. New York, MW Hyer, AM Waas. Micromechanics of linear elastic continuous fibre composites, in Comprehensive Composite Materials. Vol. 1: Fiber Reinforcements and General Theory of Composites, Eds. A Kelly, C Zweben. Elsevier, JC Halpin Affdl, JL Kardos. The Halpin-Tsai equations: A review. 1976, Vol. 16(5), pp Z Hashin, S Shtrikman. A variational approach to the theory of elastic behaviour of multiphase materials. J. Mech. Phys. Solids, 1963, Vol. 11, pp file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture29/29_10.html[8/18/2014 3:57:08 PM]

### Module 7: Micromechanics Lecture 34: Self Consistent, Mori -Tanaka and Halpin -Tsai Models. Introduction. The Lecture Contains. Self Consistent Method

Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without

### Module 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus

Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the

### Module 3: 3D Constitutive Equations Lecture 10: Constitutive Relations: Generally Anisotropy to Orthotropy. The Lecture Contains: Stress Symmetry

The Lecture Contains: Stress Symmetry Strain Symmetry Strain Energy Density Function Material Symmetry Symmetry with respect to a Plane Symmetry with respect to two Orthogonal Planes Homework References

### Module 5: Laminate Theory Lecture 19: Hygro -thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects

Module 5: Laminate Theory Lecture 19: Hygro -thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the

### Module 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations

Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates Cross-Ply Laminates Specially Orthotropic Laminates Examples Homework References

### ME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites

ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress-

### Analysis of high loss viscoelastic composites

Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science

### DEVELOPMENT OF A MICROMECHANICAL MODEL IN INTERACTION WITH PARAMETERS RELATED TO THE MICROSTRUCTURE OF CARBON/EPOXY COMPOSITES

ECCM16-16 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 22-26 June 2014 DEVELOPMENT OF A MICROMECHANICAL MODEL IN INTERACTION WITH PARAMETERS RELATED TO THE MICROSTRUCTURE OF CARBON/EPOXY

### Chapter 3. Load and Stress Analysis

Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3

### Advanced Structural Analysis EGF Cylinders Under Pressure

Advanced Structural Analysis EGF316 4. Cylinders Under Pressure 4.1 Introduction When a cylinder is subjected to pressure, three mutually perpendicular principal stresses will be set up within the walls

### Prediction of Elastic Constants on 3D Four-directional Braided

Prediction of Elastic Constants on 3D Four-directional Braided Composites Prediction of Elastic Constants on 3D Four-directional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,

### Lectures on. Constitutive Modelling of Arteries. Ray Ogden

Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics

### MATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f

MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown

### MATERIAL ELASTIC ANISOTROPIC command

MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The

### Lecture 15 Strain and stress in beams

Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME

### L e c t u r e. D r. S a s s a n M o h a s s e b

The Scaled smteam@gmx.ch Boundary Finite www.erdbebenschutz.ch Element Method Lecture A L e c t u r e A1 D r. S a s s a n M o h a s s e b V i s i t i n g P r o f e s s o r M. I. T. C a m b r i d g e December

### CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES

CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric

### Module III - Macro-mechanics of Lamina. Lecture 23. Macro-Mechanics of Lamina

Module III - Macro-mechanics of Lamina Lecture 23 Macro-Mechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the

### Module 1. Lecture 1. References:

Module 1 Lecture 1 o MF Ashby. Technology of 1990s: Advanced materials and predictive design. Phil. Trans. R. Soc. Lond. A. 1987; Vol. 322, pp. 393-407. o JY Lund, JP Byrne. Leonardo Da Vinci's tensile

### Aspect Ratio Requirements for Nanotube-Reinforced, Polymer-Matrix Composites

Aspect Ratio Requirements for Nanotube-Reinforced, Polymer-Matrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a

### Module 4: Behaviour of a Laminae-II. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites

Module 4: Behaviour of a Laminae-II Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties

### Micromechanical analysis of FRP hybrid composite lamina for in-plane transverse loading

Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382-390 Micromechanical analysis of FRP hybrid composite lamina for in-plane transverse loading K Sivaji Babu a *, K Mohana

### Exercise: concepts from chapter 8

Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic

### A simple plane-strain solution for functionally graded multilayered isotropic cylinders

Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000-000 1 A simple plane-strain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The

### The Rotating Inhomogeneous Elastic Cylinders of. Variable-Thickness and Density

Applied Mathematics & Information Sciences 23 2008, 237 257 An International Journal c 2008 Dixie W Publishing Corporation, U. S. A. The Rotating Inhomogeneous Elastic Cylinders of Variable-Thickness and

### MATERIAL PROPERTIES. Material Properties Must Be Evaluated By Laboratory or Field Tests 1.1 INTRODUCTION 1.2 ANISOTROPIC MATERIALS

. MARIAL PROPRIS Material Properties Must Be valuated By Laboratory or Field ests. INRODUCION he fundamental equations of structural mechanics can be placed in three categories[]. First, the stress-strain

### Module 3 : Equilibrium of rods and plates Lecture 15 : Torsion of rods. The Lecture Contains: Torsion of Rods. Torsional Energy

The Lecture Contains: Torsion of Rods Torsional Energy This lecture is adopted from the following book 1. Theory of Elasticity, 3 rd edition by Landau and Lifshitz. Course of Theoretical Physics, vol-7

### International Journal of Engineering Science

International Journal of Engineering Science 63 (2013) 1 9 Contents lists available at SciVerse ScienceDirect International Journal of Engineering Science journal homepage: www.elsevier.com/locate/ijengsci

### ME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)

ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,

### ANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULL-OUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES

Advanced Composite Letters, Vol. 9, No. 6, 373-383 000 Full Article ANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULL-OUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES John A. Nairn Material

### Stiffness Predictions for Unidirectional Short-Fiber Composites: Review and Evaluation

Stiffness Predictions for Unidirectional Short-Fiber Composites: Review and Evaluation Charles L. Tucker III Department of Mechanical and Industrial Engineering University of Illinois at Urbana-Champaign

### TABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA

Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1

### Department of Mechanical Engineering, National Institute of Technology Rourkela, Rourkela , India

Composites, Article ID 629175, 12 pages http://dx.doi.org/10.1155/2014/629175 Research Article Effect of Fiber Geometry and Representative Volume Element on Elastic and Thermal Properties of Unidirectional

### MODELLING THE THERMOELASTIC PROPERTIES OF SHORT FIBRE COMPOSITES WITH ANISOTROPIC PHASES

MODELLING THE THERMOELASTIC PROPERTIES OF SHORT FIBRE COMPOSITES WITH ANISOTROPIC PHASES P.J.Hine*, C.D.Price*, B.Whiteside \$, A.M.Cunha # and I.M.Ward* * - IRC in Polymer Science and Technology, University

### Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina

Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic

### Most of the material in this package is based on a recently published book. This is:

Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Pre-knowledge It is assumed that the student is familiar with simple concepts of mechanical

MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha

### Fracture Mechanics of Composites with Residual Thermal Stresses

J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate

### EVALUATION OF EFFECTIVE MECHANICAL PROPERTIES OF COMPLEX MULTIPHASE MATERIALS WITH FINITE ELEMENT METHOD

U.P.B. Sci. Bull., Series D, Vol. 79, Iss. 3, 2017 ISSN 1454-2358 EVALUATION OF EFFECTIVE MECHANICAL PROPERTIES OF COMPLEX MULTIPHASE MATERIALS WITH FINITE ELEMENT METHOD Mohamed said BOUTAANI 1, Salah

### An integrated approach to the design of high performance carbon fibre reinforced risers - from micro to macro - scale

An integrated approach to the design of high performance carbon fibre reinforced risers - from micro to macro - scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi

### Computational Analysis for Composites

Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics

### Micromechanics Analysis of Fiber Reinforced Composite

Micromechanics Analysis of Fiber Reinforced Composite Paresh K Katariya Student, ME-CAD/CAM, Department of mechanical engineering, Shree S ad Vidya Mandal Institute of Technology, Bharuch, Gujarat, India

### TRESS - STRAIN RELATIONS

TRESS - STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple

### MESH MODELING OF ANGLE-PLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP

16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLE-PLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic

### 4. BEAMS: CURVED, COMPOSITE, UNSYMMETRICAL

4. BEMS: CURVED, COMPOSITE, UNSYMMETRICL Discussions of beams in bending are usually limited to beams with at least one longitudinal plane of symmetry with the load applied in the plane of symmetry or

### STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS

1 UNIT I STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define: Stress When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The

### Chapter 3. Load and Stress Analysis. Lecture Slides

Lecture Slides Chapter 3 Load and Stress Analysis 2015 by McGraw Hill Education. This is proprietary material solely for authorized instructor use. Not authorized for sale or distribution in any manner.

### USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE

Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and

### Practice Final Examination. Please initial the statement below to show that you have read it

EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use

### Example-3. Title. Description. Cylindrical Hole in an Infinite Mohr-Coulomb Medium

Example-3 Title Cylindrical Hole in an Infinite Mohr-Coulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elasto-plastic

### ROTATING RING. Volume of small element = Rdθbt if weight density of ring = ρ weight of small element = ρrbtdθ. Figure 1 Rotating ring

ROTATIONAL STRESSES INTRODUCTION High centrifugal forces are developed in machine components rotating at a high angular speed of the order of 100 to 500 revolutions per second (rps). High centrifugal force

### PHASE VELOCITY AND ATTENUATION OF SH WAVES IN A FIBER-

PHASE VELOCITY AND ATTENUATION OF SH WAVES IN A FIBER- REINFORCED COMPOSITE Ruey-Bin Yang and Ajit K. Mal Department of Mechanical, Aerospace and Nuclear Engineering University of California, Los Angeles,

### A note on finite elastic deformations of fibre-reinforced non-linearly elastic tubes

Arch. Mech., 67, 1, pp. 95 109, Warszawa 2015 Brief Note A note on finite elastic deformations of fibre-reinforced non-linearly elastic tubes M. EL HAMDAOUI, J. MERODIO Department of Continuum Mechanics

### A parametric study on the elastic-plastic deformation of a centrally heated two-layered composite cylinder with free ends

Arch. Mech., 68, 3, pp. 03 8, Warszawa 06 A parametric study on the elastic-plastic deformation of a centrally heated two-layered composite cylinder with free ends F. YALCIN ), A. OZTURK ), M. GULGEC 3)

### CHAPTER 4 MODELING OF MECHANICAL PROPERTIES OF POLYMER COMPOSITES

CHAPTER 4 MODELING OF MECHANICAL PROPERTIES OF POLYMER COMPOSITES 4. Introduction Fillers added to polymer matrices as additives are generally intended for decreasing the cost (by increase in bulk) of

### QUESTION BANK Composite Materials

QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.

### A Comparative Study of Analytical and Numerical Evaluation of Elastic Properties of Short Fiber Composites

IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS A Comparative Study of Analytical and Numerical Evaluation of Elastic Properties of Short Fiber Composites To cite this article:

### THERMOELASTIC ANALYSIS OF THICK-WALLED FINITE-LENGTH CYLINDERS OF FUNCTIONALLY GRADED MATERIALS

Journal of Thermal Stresses, 28: 391 408, 2005 Copyright # Taylor & Francis Inc. ISSN: 0149-5739 print/1521-074x online DOI: 10.1080/01495730590916623 THERMOELASTIC ANALYSIS OF THICK-WALLED FINITE-LENGTH

### 2.2 Relation Between Mathematical & Engineering Constants Isotropic Materials Orthotropic Materials

Chapter : lastic Constitutive quations of a Laminate.0 Introduction quations of Motion Symmetric of Stresses Tensorial and ngineering Strains Symmetry of Constitutive quations. Three-Dimensional Constitutive

### Development of a code to generate randomly distributed short fiber composites to estimate mechanical properties using FEM

International Journal of Theoretical and Applied Mechanics. ISSN 0973-6085 Volume 12, Number 4 (2017) pp. 863-872 Research India Publications http://www.ripublication.com Development of a code to generate

### 3D Elasticity Theory

3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.

### Composite Structures. Indian Institute of Technology Kanpur

Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2

### CHEM-C2410: Materials Science from Microstructures to Properties Composites: basic principles

CHEM-C2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and

### A micromechanical model for effective elastic properties of particulate composites with imperfect interfacial bonds

International Journal of Solids and Structures 42 (2005) 4179 4191 www.elsevier.com/locate/ijsolstr A micromechanical model for effective elastic properties of particulate composites with imperfect interfacial

### Composite models 30 and 131: Ply types 0 and 8 calibration

Model calibration Composite Bi-Phase models 30 and 3 for elastic, damage and failure PAM-CRASH material model 30 is for solid and 3 for multi-layered shell elements. Within these models different ply types

### Predicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics

Predicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics Neelam Mishra 1, and Kaushik Das *1 1 School of Minerals Metallurgical and Materials Engineering, Indian

### Effects of Random Cross-Sectioned Distributions, Fiber Misalignment and Interphases in Three- Dimensional Composite Models on Transverse Shear Modulus

University of South Florida Scholar Commons Graduate Theses and Dissertations Graduate School January 2012 Effects of Random Cross-Sectioned Distributions, Fiber Misalignment and Interphases in Three-

### Distributed: Wednesday, March 17, 2004

MASSACHUSETTS INSTITUTE OF TECHNOLOGY DEPARTMENT OF MECHANICAL ENGINEERING CAMBRIDGE, MASSACHUSETTS 019.00 MECHANICS AND MATERIALS II QUIZ I SOLUTIONS Distributed: Wednesday, March 17, 004 This quiz consists

### Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach

Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Now-a-days,

### Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",

Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity

### Tuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE

1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & Free-Body Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for

### XI. NANOMECHANICS OF GRAPHENE

XI. NANOMECHANICS OF GRAPHENE Carbon is an element of extraordinary properties. The carbon-carbon bond possesses large magnitude cohesive strength through its covalent bonds. Elemental carbon appears in

### McMAT 2007 Micromechanics of Materials Austin, Texas, June 3 7, 2007

McMAT 2007 Micromechanics of Materials Austin, Texas, June 3 7, 2007 RANDOM POLYCRYSTALS OF GRAINS WITH CRACKS: MODEL OF ELASTIC BEHAVIOR FOR FRACTURED SYSTEMS James G. Berryman Earth Sciences Division

### Mechanics of Materials II. Chapter III. A review of the fundamental formulation of stress, strain, and deflection

Mechanics of Materials II Chapter III A review of the fundamental formulation of stress, strain, and deflection Outline Introduction Assumtions and limitations Axial loading Torsion of circular shafts

### Elements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004

Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic

### Fig. 1. Circular fiber and interphase between the fiber and the matrix.

Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In

### Enhancing Prediction Accuracy In Sift Theory

18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department

### CHEM-E2200: Polymer blends and composites Fibre architecture and principles of reinforcement

CHEM-E2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle

### 3 2 6 Solve the initial value problem u ( t) 3. a- If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1

Math Problem a- If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1 3 6 Solve the initial value problem u ( t) = Au( t) with u (0) =. 3 1 u 1 =, u 1 3 = b- True or false and why 1. if A is

### Evaluation of Effective Elastic Moduli Using Micromechanics

IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Evaluation of Effective Elastic Moduli Using Micromechanics To cite this article: Misba Mehdi Mrs. et al 2018 IOP Conf. Ser.:

### Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate

Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical

### An orthotropic damage model for crash simulation of composites

High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures

### Understand basic stress-strain response of engineering materials.

Module 3 Constitutive quations Learning Objectives Understand basic stress-strain response of engineering materials. Quantify the linear elastic stress-strain response in terms of tensorial quantities

### MECHANICS OF MATERIALS

2009 The McGraw-Hill Companies, Inc. All rights reserved. Fifth SI Edition CHAPTER 3 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Torsion Lecture Notes:

### Samantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2

Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force

Frequently Asked Questions Why do we have to make the assumption that plane sections plane? How about bars with non-axis symmetric cross section? The formulae derived look very similar to beam and axial

### Numerical evaluation of effective material properties of randomly distributed short cylindrical fibre composites

Computational Materials Science 39 (2007) 198 204 www.elsevier.com/locate/commatsci Numerical evaluation of effective material properties of randomly distributed short cylindrical fibre composites S. Kari

### Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37

Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREE-DIMENSIONAL, TIME- DEPENDENT, NON-LINEAR, UNI-DIRECTIONAL

### Multiscale Approach to Damage Analysis of Laminated Composite Structures

Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University

### Lecture 8. Stress Strain in Multi-dimension

Lecture 8. Stress Strain in Multi-dimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]

### Mechanics of Materials and Structures

Journal of Mechanics of Materials and Structures ON SMALL AZIMUTHAL SHEAR DEFORMATION OF FIBRE-REINFORCED CYLINDRICAL TUBES Mohamed A. Dagher and Kostas P. Soldatos Volume 6, No. 1-4 January June 2011

### MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS

MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is

### DEVELOPMENT OF SOPHISTICATED MATERIALS USING THE COMPUTER SIMULATION

7 th INTERNATIONAL MULTIDISCIPLINARY CONFERENCE Baia Mare, Romania, May 17-18, 2007 ISSN-1224-3264 DEVELOPMENT OF SOPHISTICATED MATERIALS USING THE COMPUTER SIMULATION Zuzana MURČINKOVÁ Ing. Zuzana MURČINKOVÁ,

### Crash and Impact Simulation of Composite Structures by Using CAE Process Chain

Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de

### Course No: (1 st version: for graduate students) Course Name: Continuum Mechanics Offered by: Chyanbin Hwu

Course No: (1 st version: for graduate students) Course Name: Continuum Mechanics Offered by: Chyanbin Hwu 2011. 11. 25 Contents: 1. Introduction 1.1 Basic Concepts of Continuum Mechanics 1.2 The Need

### MECHANICS OF MATERIALS

GE SI CHAPTER 3 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Torsion Lecture Notes: J. Walt Oler Texas Tech University Torsional Loads on Circular Shafts

### USE OF A LINEAR VISCOELASTIC CONSTITUTIVE LAW TO MODEL THE TIME DEPENDENT BEHAVIOUR OF ORTHOTROPIC GLASSFIBRE REINFORCED PLASTIC

USE OF A LINEAR VISCOELASTIC CONSTITUTIVE LAW TO MODEL THE TIME DEPENDENT BEHAVIOUR OF ORTHOTROPIC GLASSFIBRE REINFORCED PLASTIC Roland. M. Hinterhoelzl 1, Guenther Schullerer 1, Kurt Moser 1 1 Institut

### LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS

XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds